Chemical and structural analysis on magnetic tunnel junctions using a
decelerated scanning electron beam
Edward Jackson,1 Mingling Sun,2 Takahide Kubota,2,3 Koki Takanashi 2,3 and Atsufumi Hirohata 1, *
1 Department of Electronic Engineering, University of York, Heslington, York YO10 5DD,
2 Institute for Materials Research, Tohoku University, 2-1-1 Katahira, Sendai 980-8577,
3 Center for Spintronics Research Network, Tohoku University, 2-1-1 Katahira, Sendai
* e-mail: email@example.com
Current information technology relies on the advancement of nanofabrication
techniques. For instance, the latest computer memories and hard disk drive read
heads are designed with a 12 nm node and 20 nm wide architectures,
respectively. With matured nanofabrication processes, a yield of such
nanoelectronic devices is typically up to about 90%. To date the yield has been
compensated with redundant hardware and software error corrections. In the
latest memories, approximately 5% redundancy and parity bits for error
corrections are used, which increase the total production cost of the devices.
This means the yield directly affects the device costs. It is hence critical to
increase the yield in nanofabrication. In this paper, we have applied our recently
developed method to image buried interfaces in combination with chemical
analysis to evaluate magnetic tunnel junctions and have revealed their different
magnetoresistance ratios caused by the presence of materials formed at the
junction edges. The formation of these materials can be avoided by optimising
the junction patterning process to remove residual carbon introduced from
resist. Our imaging method with chemical analysis have demonstrated a
significant potential for the improvement of junction performance, resulting in
higher yields. This can be used as a quality assurance tool in a nanoelectronic
device production line.
Human beings have been reported to have created 4.4 ZB data in 2013 and are expected to create 44 ZB in 20201.. Such drastic increase of 40% annually in the digital universe is based on the development of nanoelectronic devices, e.g., data processing chips with a 12 nm node and hard disk drives with a 20 nm wide read heads. The latest development on 3-dimensional (3D) NAND flash memories have also achieved 512 Gbit on a single Si die with the area of around 130 mm2 independently demonstrated by Toshiba-Western Digital and Samsung2.. However, the miniaturisation of the nanoelectronic devices have in turn reduced their yields due to defects and non-uniformity induced during their complicated fabrication processes. The yield (Y) can be
(Number of working devices on a die
(Number of total devices fabricated on a die
). (1) It is widely known that the final device yield can be approximately 90% for a series of optimised processes in nanoelectronics. The exponential yield model gives the following relationship:
where A and D represent area and defect density of a device fabricated, respectively. In Eq. (2), if D is assumed to be the same on a die, the reduction in A increases Y. In
reality, the milling or etching processes to fabricate a nanometre-scale junctions induce additional edge defects, such as redeposition of materials and edge roughness distributions, which increases D.
In order to compensate a 90% yield to reduce the cost of the device production, hardware redundancy3. has been implemented in a device. For example, one of the most common redundancy in a memory is a built-in self-repair technique, which consumes about 5% of the memory. It runs a test of the memory functionality and then analyse redundancy, followed by the allocation of redundant memories for the
function is implemented to physically repair the broken section. Software error corrections4. are also widely utilised in a device input/output interface with additional parity bits. The hardware solution is one-time repair requiring additional technology but it can repair the device in a short time. On the other hand, the software solution is multiple-time repair with almost no design overhead but it can repair only limited latent defects requiring additional processing data time. Therefore, it is crucial to develop a revolutionary method to optimise the device structures to achieve a yield of almost 100%.
Further improvement of the yield requires intensive process optimisation fed back from techniques such as cross-sectional transmission electron microscopy (TEM) imaging etc. TEM observation allows for atomic scale studies into device structure, but the images may not be representative of the device interfaces because of the destructive sample preparation inducing additional strain and defects to the interfaces. Other options are to investigate devices with photoemission electron microscopy (PEEM). This relies on EM radiation to excite or liberate electrons which then provide information about the structure. Unfortunately this is very surface sensitive so is not suited for these kind of studies without intensive sample preparation similar to TEM. In this study, we have demonstrated chemical analysis alongside decelerated electron-beam imaging for buried magnetic tunnel junctions (MTJs) to reveal the origin of the reduction in tunnelling magnetoresistance (TMR) ratios for some of the MTJs. We have recently developed a new non-destructive method to image buried junctions using a decelerated electron-beam5.. By using a precisely controlled beam we have managed to image MTJs below an 80-nm-thick Au electrode, allowing a correlation between the junction images and their magnetic transport properties to be made. The reduction in their TMR ratios have been found to be induced by the formation of aluminium carbide in resist during Ar-ion milling to pattern MTJ pillars. This has been fed back to the fabrication process for the optimisation and can be applicable for the other nanoelectronic devices.
Magnetic transport properties. Many MTJs, consisting of MgO(001)//Cr (80)/Pd (5)/Co2Fe0.4Mn0.6Si (30)/MgO (2)/Co0.5Fe0.5 (5)/IrMn3 (10)/Ru (7)/Cr (5)/Au (80) (thickness in nm), were measured by a four-terminal method. The results of these measurements are shown in Supplementary Table ST1. Two distinctive groups of MTJs were found in terms of their TMR ratios: (i) A large TMR ratio of over 80% and (ii) a small TMR ratio of about 20% as shown in Fig. 1. Their resistance-area product (RA)
were also found to be as different as 4.2104µm2 for the group (i) and 4.7103µm2 for the group (ii). The average difference between these groups was approximately one order of magnitude.
Figure 1 Magnetic tunnel junctions studied. Multilayered structure of MgO(001)//Cr (80)/Pd (5)/Co2Fe0.4Mn0.6Si (30)/MgO (2)/Co0.5Fe0.5 (5)/IrMn3 (10)/Ru (7)/Cr (5)/Au (80) (thickness in nm). The multilayers were patterned into magnetic tunnel junctions (MTJs) by photolithography and Ar-ion milling. MTJs were measured by a four-terminal method, showing a typical tunnelling magnetoresistance (TMR) ratio and
resistance-area product (RA) of a, 110% and 3.8104 µm2 and b, 18% and 4.7103 µm2,
respectively. In the supplementary section there are also results shown from a similar set of devices where CFMS = 5 nm.
Electron flight simulations. Electron flights in a multilayered structure were simulated at a series of decelerated electron-beam between 9 and 12 kV using CASINO6.. The histograms from these simulations are shown in supplementary Fig. S2. Here, the Co2Fe0.4Mn0.6Si (CFMS)/MgO/CoFe junctions were the layers of interest to correlate any potential defects with the above mentioned TMR reduction. All the layer compositions and their thicknesses were used to simulate the electron flights in the entire multilayers. As shown in Fig. 2a using a 9-kV electron beam, the CASINO simulations confirmed almost 0.002% of the electrons to penetrate into the bottom CFMS layer, while 0.001% and 0.006% were to penetrate the MgO and CoFe layers, respectively. On the other hand, a 12-kV electron beam was calculated to penetrate the CFMS, MgO and CoFe layers by 0.13%, 0.04% and 0.19%, respectively. These simulations gave over 4000% of changes in the penetration probabilities within the CFMS/MgO/CoFe junctions with these decelerated electron-beam voltages (Vacc).
Figure 2 Simulations and SEM images of MTJs with decelerated electron beam.
Interaction-volume simulations to estimate the penetration depth for 15 µm15 µm MTJs with 30nm CFMS as shown in Fig. 1 at decelerated electron-beam voltages (Vacc) of a, 9 and b, 12 kV. The red traces represent the backscattered electron’s (BSE) path.
Corresponding scanning electron microscopy (SEM) images are taken by the upper electron detector (UED) with the BSE mode at Vacc=10.5 and 11 kV. These two images
are subtracted as shown in c, for an MTJ with a large TMR ratio (83%) and d, for an MTJ with a small TMR ratio (18%). Note the line observed in Fig. 2c is a scratch made
during the device transfer into SEM.
Imaging with decelerated electron beam. Based on the above simulations, SEM images of the MTJs were taken at the decelerated voltages of 9 and 12 kV as shown in Supplementary Fig. S1. Since our simulations did not take additional parameters, such as film densities, defects and interfacial roughness, further optimisation of Vacc for imaging was carried out with these voltages. This involved taking a series of images at voltages indicated by the previous simulations. The images that provided the greatest contrast in regions of interest were chosen. A set of two representative images were
selected to be taken at Vacc=10.5 and 11 kV. The former image taken at Vacc=10.5 kV should be predominantly sensitive to any defects above the MgO/CoFe interfaces, while the latter one taken at Vacc=11 kV should be primarily sensitive to any defects above the CFMS/MgO interfaces. Hence, by subtracting these two images, one should be able to reconstruct an image representing any defects in the vicinity of the MgO tunnelling barrier.
Figures 2c and 2d shows the subtracted SEM images taken between Vacc=10.5 and 11 keV for the groups (i) and (ii), respectively. It should be noted that both images do not have any defects within the MTJ pillars, which can be observed as grey regions without generating backscattered electrons (BSEs) as imaged previously, suggesting the multilayers are free from interfacial defects. Hence the focus is given to the edges of the pillars. Both images show ~300 nm wide gradient at the edges of the MTJ pillars. This gradient region indicates that the cross-section of the pillars has a shape of trapezium due to the patterning process using Ar-ion milling. In addition, Figure 2d possesses wider edges at the left edge especially, which suggests the edge may suffer from extra materials redeposited during the milling process. It is important to note that at this stage the change in edge width could just been down to a difference in the incident angle of the Ar-ion beam used to mill the pillars. Chemical analysis done alongside this comparison can help reveal the origin of this oddity.
Chemical analysis. In order to clarify the origin of the materials attached at the edge, energy dispersive X-ray spectroscopy (EDX) analysis was performed on these two distinctive groups of MTJs. Figure 3, with more examples in supplementary fig S3, shows the EDX signals for the group (i) with large TMR ratios measured at the electron-beam energy between 0.1 and 10 kV and the associated mapping against elements of C, Al, Au and Ru. The strongest signal is from the Au top electrodes, followed by the Al-O insulating layer surrounding the MTJ pillars due to their large volume. Additional minor signals from C, Mg and Ru are appeared in the signal. The EDX mapping confirms that Au is distributed over the surface of the MTJ devices. Al is found to exist only outside the MTJ pillar, while Ru is visible only within the MTJ pillar as expected. It is important to note that C has almost no intensity over the device,
indicating no residual resist after the device fabrication and no C-based contamination formed during the analysis.
Figure 3 Chemical analysis on an MTJ with a large TMR ratio. Energy dispersive X-ray spectroscopy (EDX) profile for the electron-beam energy between 0.1 and 10 kV for the MTJ. SEM image taken at 10 kV and the corresponding EDX maps are shown for C, Al, Au and Ru.
Figure 4, with further examples in supplementary fig. S4, on the other hand, shows the EDX signals for the group (ii) with almost no TMR ratios measured at the electron-beam energy between 0.1 and 10 kV and the associated mapping against elements of C, Al, Au and Ru. The strongest signal is again from the Au top electrodes, followed by the Al-O insulating layers surrounding the MTJ pillars due to their large volume. Additional minor signals from C, Mg and Ru are appeared in the signal as seen in Fig. 3. In the corresponding EDX mapping, Ru is visible only within the MTJ pillar as expected. However, the other elements in EDX mapping shows different results from those in Fig. 3. In Fig. 4, Au distributed over the surface of the MTJ devices except the
bottom right edge of the pillar. In this region, Al is found to be concentrated more strongly than that outside the MTJ pillar. Similarly, C is only detected in the same region. This may indicate the formation of an aluminium carbide, such as Al4C3, at the edge of the MTJ nanopillar. Al4C3 is known to be formed by the reduction of Al-O at high temperature (~2000ºC). This may suggest residual resist after the Ar-ion milling process may react with Al-O during the Al-O sputtering process. Hence, the resistivity
of Al4C3 has been reported to be 102 cm,7. which is much smaller than that of MgO, 1012cm. The formation of any aluminium carbides at the edge of a MTJ pillar would cause current shunting through the particles, reducing the corresponding TMR ratio and RA.
Figure 4 Chemical analysis on an MTJ with a small TMR ratio. Energy dispersive X-ray spectroscopy (EDX) profile for the electron-beam energy between 0.1 and 10 kV for the MTJ. SEM image taken at 10 kV and the corresponding EDX maps are shown for C, Al, Au and Ru.
By comparing the subtracted SEM image and EDX mapping in Figs. 2c and 3, the group (i) with large TMR ratios is found to possess smooth interfaces and clean edges. This ensures ideal magnetic transport, achieving the TMR ratio over 80%. On the other hand, Figures 2d and 4 confirm smooth interfaces in the MTJ pillars but with aluminium carbide formation at the edge of the pillars. This introduces a shorting current path, reducing the TMR ratio close to zero. These differences are consistent with the reduction in RA by one order of magnitude. The aluminium carbide particles at the MTJ edges are formed by Al-O sputtering onto the residual resist containing carbon. Similar aluminium carbide particles are observed in the other MTJs in the group (ii). The average size of the smallest features are measured to be around 900 nm. By using the
resistivity of Al4C3, RA through such a particle is estimated to be 9105 µm2. In the case of the 5 nm CFMS devices we managed to improve the yield from 21% to 36% by reducing the beam current during the Al-O deposition, with details discussed in the supplementary section and results shown in ST3. The EDX mapping with decelerated electron-beam imaging therefore allow further process optimisation of junction fabrication to sustain the advancement in their density and functionality at low cost.
Device fabrication. Multilayers, consisting of Cr (80)/Pd (5)/Co2Fe0.4Mn0.6Si (5 or 30)/MgO (2)/Co0.5Fe0.5 (5)/IrMn3 (10)/Ru (7) (thickness in nm), were grown on MgO(001) substrates at room temperature using an ultrahigh vacuum (UHV) sputtering system (ULVAC, MPS series)8.. After the deposition of the CFMS layer, the entire stack was annealed at 400ºC for 20 minutes in the UHV system to crystallise the CFMS Heusler alloy layer into the perfectly-ordered L21 phase.
The structure listed above, and shown in Fig. 1, was chosen to maximise TMR effects and also allow for simple transport measurements. The bottom Cr and Pd layers act simultaneously as seed layers, to promote the L21 phase, and electrodes for measurement. The CFMS is the free layer, with the CoFe acting as it’s reference layer and the MgO as the tunnel barrier. The IrMn3 provides exchange bias, fixing the
reference layer. Finally the Ru, Cr and Au act as both capping layers and lead electrodes for the system.
The multilayered stacks were then patterned into MTJs with their area between 10
µm10 µm and 50 µm50 µm using photolithography and Ar-ion milling. Here, photoresist of AZ5214E (Micro Chemicals) with typical thickness of 1.4 µm was spin-coated on the multilayers to create positive patterns of bottom electrodes. The patterns were then milled by Ar+ ions (Hakuto, 10IBE), followed by the removal of the remaining resist using N-methylpyrrolidone. On these bottom electrodes, MTJ pillars were patterned using the same milling process with end-point detection just below the Pd/CFMS interfaces. The milled regions were filled with Al-O by UHV sputtering, followed by the lift-off with N-methylpyrrolidone. The top electrodes of Cr (5)/Au (80) (thickness in nm) were finally deposited by UHV sputtering through similarly made patterns by photolithography, followed by the similar lift-off process.
Magnetotransport measurement. The transport properties of the MTJs were assessed by four-terminal magnetoresistance measurements. Here, an electrical current of about 100 µA and an external magnetic field of up to ± 50 mT along the <110> direction of the CFMS layer were applied during the measurements at room temperature. The details of the magnetotransport properties have been published elsewhere11..
SEM observation. In the JSM-7800F Prime SEM9., an upper electron detector (UED) is located above the lens and two additional detectors, a retractable backscattered electron detector (BED) and a lower electron detector (LED), are installed just above the sample space. The UED becomes sensitive to reflected electrons from the specimen with energies above 10 eV when a bias voltage (V) is applied to the energy filter beneath, while the USD senses those below 1 eV. These detection modes with energy deceleration in the range between +500 eV and -2 keV can be achieved coincidently. In addition, the acceleration voltage for the electron-beam can be controlled between 10 and 30 kV10.. Based on such controllability, almost 0.7-nm resolution is guaranteed at the effective electron-beam landing voltages of both 1 and 5 kV at the specimen by the manufacturer.
Data availability. The data that support the findings of this study are available from the corresponding author upon request.
2. IEEE International Solid-State Circuits Conference, 5-9 February 2017, San Francisco, CA, USA.
3. Gonzales, M. A., Holman, T. J. and Stolt, P. F. Method and apparatus for automatically scrubbing ECC errors in memory via hardware. US Patent US6101614 A (2000).
4. Oshaki, A. and Yamada, A. Memory device to detect and compensate for defective memory cells. US Patent US5477492 A (1995).
5. Hirohata, A., Yamamoto, Y., Murphy, B. A. and Vick, A. J. Non-destructive imaging of buried electronic interfaces using a decelerated scanning electron beam. Nature Commun.7, 12701 (2016).
6. Drouin, D., Couture, A. R., Joly, D., Tastet, X., Aimez, V. and Gauvin, R. CASINO V2.42 – A fast and easy-to-use modeling tool for scanning electron microscopy and microanalysis users. Scanning29, 92 (2007).
7. King, W. R. and Dorward, R. C. Electrical Resistivity of Aluminum Carbide at 990– 1240 K. J. Electrochem. Soc.132, 2 (1985).
8. Kubota, T., Kamada, T., Kim, J., Tsukamoto, A., Takahasi, S., Sonobe, Y. and Takanashi, K. Interface Magnatic Anisotropy of Pd/Co2FexMn1-xSi/MgO Layered Structures. Mater. Trans.57, 773 (2016).
9. Jackson, E., DuttaGupta, S., Fukami, S., Ohno, H. and Hirohata, A. Imaging defects in magnetic multilayers using scanning electron microscopy to correlate their magneto-transport properties. Appl. Phys. Lett. (to be submitted).
10. Hirohata, A. Method of imaging defects using a scanning electron microscope. British patent GB1522137.7 (pending).
11. Sun, M., Kubota, T., Takahashi, S., Kawato, Y., Sonobe, Y., and Takanashi, K., Buffer layer dependence of magnetoresistance effects in Co2Fe0.4Mn0.6Si/MgO/Co50Fe50 tunnel junctionst. AIP Advances 8, 055902 (2018).
The authors thank the technical support for the SEM imaging by JEOL UK. This work is partially funded by the Engineering and Physical Sciences Research Council (EPSRC, EP/M02458X/1) as well as a HARFIR (Heusler alloy replacement for Iridium) project by the European Commission under the 7th Framework Programme (FP7-NMP-2013-EU-Japan, Grant Agreement No: NMP3-SL-2013-604398) and by the Japan Science and Technology Agency through its Strategic International Collaborative Research Program, also thanks should be made to the JSPS Core-to-Core project.
E.J. performed the SEM observation with the controlled electron-beam deceleration and the associated simulations. M.S., T.K. and K.T. fabricated the junctions and carried out the magnetic transport measurements. A.H. conceived the experiment and analysed the SEM images with E.J. All authors contributed to the interpretation of the results and writing of the manuscript.
Competing financial interests
The authors declare no competing financial interests.
Figure S1 shows raw SEM images taken at the electron-beam acceleration voltages between 9 and 12 kV. As seen in Fig. S1a, there are two circular defects observed in the middle of the MTJ nanopillar, which become significant in Fig. S1b but diminish in Figs. S1c and d. By making electron flight simulations on these acceleration voltages as shown in Fig. S2, the defects are formed in the layers between the top Cr and CoFe, which may not change the magnetic transport properties across CoFe/MgO/Co2Fe0.4Mn0.6Si (CFMS). Additional vertical stripe features are seen in Fig. S1. Since these stripe features are observed in all four SEM images, they may be induced by the initial interface between the MgO substrate and the Cr seed layer. Hence, no major defects are formed across the CFMS/MgO/CoFe interfaces. These images are subtracted for comparison as discussed in the main text, to ascertain which voltages should be utilised for more intensive analysis of the interface of interest, the MgO barrier.
Figure S1: Decelerated beam images. A series of images taken of one of the magnetic tunnel junctions, consisting of MgO(001)//Cr (80)/Pd (5)/Co2Fe0.4Mn0.6Si (5)/MgO (2)/Co0.5Fe0.5 (5)/IrMn3 (10)/Ru (7)/Cr (5)/Au (80) (thickness in nm). This device is 15 µm 15 µm imaged at the acceleration beam voltages of a, 9, b, 9.5, c, 10, d, 10.5, e, 11 and f, 12 kV.
As can be seen in these histograms the number of electrons interacting with the areas of interest (MgO/CFMS/CoFe) greatly increase with increasing acceleration voltages. In this system the 80nm Au cap acts as a very large barrier for electrons. As the voltage increases larger numbers can overcome this barrier drastically increasing the number of BSE interactions.
Figure S2: Decelerated beam simulations. A series of histograms of backscattered
electrons to be generated from a magnetic tunnel junctions, consisting of MgO(001)//Cr (80)/Pd (5)/Co2Fe0.4Mn0.6Si (5)/MgO (2)/Co0.5Fe0.5 (5)/IrMn3 (10)/Ru (7)/Cr (5)/Au (80) (thickness in nm) at the acceleration beam voltages of a, 9, b, 9.5, c, 10, d, 10.5, e, 11 and f, 12 kV. The remainder of the BSEs are found in the gold capping layer.
Figure S3: High TMR Pillar EDX. Further EDX profiles for a high TMR pillar. SEM image taken at 10 kV and the corresponding EDX maps are shown for C, Al, Au and Ru. In this case strong carbon surface contaminants can be seen, but despite this the same structures appear. Ru is confined to the pillar and Al is kept outside of it as expected.
Figure S4: low TMR Pillar EDX. Further EDX profiles for a low TMR pillar. SEM image taken at 10 kV and the corresponding EDX maps are shown for C, Al, Au and Ru. In this case the Al’s most well defined feature is along the edge of the pillar, which can be correlated to the SEM image and the lower concentration of Au.
To test the hypothesis that aluminium carbide formation during the deposition of aluminium oxide is reducing the yield of the devices studied a second set of similar samples were produced. In this set the aluminium oxide was deposited at 60% of the original current. In the 1st set of samples, tabulated in ST1, the yield was 69%. This was defined by the number of devices with a MR ≥ 80%, dived by the total number of devices produced (42). For the 2nd set, with a lower beam current, this yield dropped to 12%.
Size (µm2) MR(%) RA (Ωµm2)
50 x 50 80.20 2.56 x104
50 x 50 95.2 3.56 x104
50 x 50 73.2 2.02 x104
50 x 50 94.7 4.38 x104
50 x 50 87.1 3.54 x104
50 x 50 0 0
Size (µm2) MR(%)
40 x 40 86.2
40 x 40 94.8
40 x 40 92.9
40 x 40 53.2
40 x 40 83.4
40 x 40 93.8
RA (Ωµm2) 3.13 x104 3.68 x104 3.55 x104 1.25 x104 3.06 x104 3.87 x104 Size (µm2)
MR(%) RA (Ωµm2)
30 x 30 94.1 3.72 x104
30 x 30 83 2.80 x104
30 x 30 7
30 x 30 18.4 1.53 x103
30 x 30 96.4 4.19 x104
30 x 30 97.7 4.16 x104 Size (µm2)
MR(%) RA (Ωµm2)
25 x 25 28.59 8.79 x103
25 x 25 87.4 3.18 x104
25 x 25 95 3.69 x104
25 x 25 44.6 8.38 x103
25 x25 33.4 4.96 x103
25 x 25 97.7 4.06 x104 Size (µm2)
MR(%) RA (Ωµm2)
20 x 20 95.4 3.67 x104
20 x 20 96.83 3.72 x104
20 x 20 95.9 3.70 x104
20 x 20 73.5 2.19 x104
20 x 20 96.7 3.97 x104
20 x 20 95.3 3.82 x104 Size (µm2)
MR(%) RA (Ωµm2)
15 x 15 75.4 2.34 x104
15 x 15 96.8 3.52 x104
15 x 15 93.7 3.45 x104
15 x 15 91.3 3.43 x104
15 x 15 96.1 3.83 x104
15 x 15 96.5 3.78 x104 Size (µm2)
MR(%) RA (Ωµm2)
10 x 10 95.1 3.33 x104
10 x 10 94.4 3.19 x104
10 x 10 0 0
10 x 10 23.9 2.24 x103
10 x 10 44.4 5.97 x103
10 x 10 95.8 3.40 x104 Table ST1: Transport measurements for the devices with MgO(001)//Cr (80)/Pd (5)/Co2Fe0.4Mn0.6Si (30)/MgO (2)/Co0.5Fe0.5 (5)/IrMn3 (10)/Ru (7)/Cr (5)/Au (80) (thickness in nm). If the devices are grouped by their MR, either high or low, the groups will contain devices from the full range of sizes.
Size (µm2) MR(%) RA (Ωµm2)
50 x 50 34.4 3.85 x104
50 x 50 25.9 2.98 x104
50 x 50 46.5 5.05 x104
50 x 50 107.0 7.83 x104
50 x 50 38.2 4.21 x104
50 x 50 32.7 3.85 x104 Size (µm2)
MR(%) RA (Ωµm2)
40 x 40 25.7 3.14 x104
40 x 40 67.9 6.02 x104
40 x 40 23.7 3.06 x104
40 x 40 54.2 5.17 x104
40 x 40 21.3 2.53 x104
40 x 40 42.4 4.42 x104 Size (µm2)
MR(%) RA (Ωµm2)
30 x 30 8.6 1.06 x104
30 x 30 51 4.97 x104
30 x 30 32 9.86 x104
30 x 30 51.2 4.91 x104
30 x 30 38.4 4.12 x104
30 x 30 47.2 4.70 x104 Size (µm2) 25 x 25 25 x 25 25 x 25 25 x 25 25 x25 25 x 25
MR(%) RA (Ωµm2)
24.9 2.96 x104
9.6 1.27 x104
30.5 3.59 x104
8.0 8.94 x103
7.2 8.63 x103
84.9 6.33 x104 Size (µm2)
MR(%) RA (Ωµm2)
20 x 20 46.2 4.66 x104
20 x 20 63.6 5.42 x104
20 x 20 97.1 7.53 x104
20 x 20 101.4 6.62 x104
20 x 20 7.8 5.15 x103
20 x 20 83.2 6.24 x104 Size (µm2)
MR(%) RA (Ωµm2)
15 x 15 19.3 2.30 x104
15 x 15 95.0 6.99 x104
15 x 15 6
15 x 15 97.0 6.14 x104
15 x 15 46.8 4.22 x104
15 x 15 22.6 2.32 x104 Size (µm2)
MR(%) RA (Ωµm2)
10 x 10 9.7 1.11 x104
10 x 10 11.5 1.34 x104
10 x 10 6
10 x 10 72.6 4.99 x104
10 x 10 87.4 5.49 x104
10 x 10 85.2 5.50 x104 B
Size (µm2) MR(%) RA (Ωµm2)
50 x 50 95.7 5.20 x104
50 x 50 8.7 5.50 x103
50 x 50 60.4 3.83 x104
50 x 50 8.20 6.50 x103
50 x 50 15.5 1.20 x104
50 x 50 95.5 4.95 x104 Size (µm2)
MR(%) RA (Ωµm2)
40 x 40 93.3 4.90 x104
40 x 40 6.5 5.76 x103
40 x 40 95.3 4.99 x104
40 x 40 15.9 1.22 x104
40 x 40 13.7 1.14 x104
40 x 40 3.7 3.04 x103 Size (µm2)
MR(%) RA (Ωµm2)
30 x 30 92.3 4.59 x104
30 x 30 92.3 4.73 x104
30 x 30 16.9 1.39 x104
30 x 30 90.3 4.67 x104
30 x 30 90.3 4.64 x104
30 x 30 24.2 1.80 x104 Size (µm2)
MR(%) RA (Ωµm2)
25 x 25 89.0 4.66 x104
25 x 25 31.5 2.24 x104
25 x 25 91 4.63 x104
25 x 25 87.8 4.51 x104
25 x25 10.3 7.88 x103
25 x 25 90.0 4.36 x104 Size (µm2)
MR(%) RA (Ωµm2)
20 x 20 26.1 1.98 x104
20 x 20 26.2 1.88 x104
20 x 20 88.2 4.46 x104
20 x 20 85.1 4.16 x104
20 x 20 12.3 8.56 x103
20 x 20 12.4 8.92 x103 Size (µm2)
MR(%) RA (Ωµm2)
15 x 15 14.2 1.13 x104
15 x 15 12.9 6.93 x103
15 x 15 79.0 4.14 x104
15 x 15 84.3 2.56 x104
15 x 15 21.6 1.40 x104
MR(%) RA (Ωµm2)
1.85 x103 66.4 3.94 x104
79.3 2.00 x104
61.2 3.95 x104
62.0 3.90 x104
62.3 3.82 x104 Table ST2: Transport measurements for the devices with MgO(001)//Cr (20)/Ru(50)/Co2Fe0.4Mn0.6Si (5)/MgO (2)/Co0.5Fe0.5 (5)/IrMn3 (10)/Ru (7)/Cr (5)/Au (80) (thickness in nm). (A) shows the devices which had aluminium oxide deposited at 50 mA. (B) shows the devices which had aluminium oxide deposited at 30 mA.
This drop can be explained by the increase in difficulty of lift-off due to the hardening of the photoresist. This hardening occurred because the cooling of the stage was insufficient for such a long deposition time. With this in mind the CFMS = 5 nm group of samples, which are tabulated in ST2, were investigated in a similar manner. As they were shorter stacks, even at the lower deposition current they would not take long enough for the cooling to become inadequate. In this case the 1st set of samples had a yield of 21%, whilst the 2nd set had a yield of 36%. This increase demonstrates that one of the issues this structure faced was the formation of aluminium carbide, which allowed us to remove one of the problems in device fabrication. A summary of this yield test is shown in Table ST3.
Device Group 30 - 1st 30 - 2nd 5 – 1st 5 – 2nd
(mA) 50 30 50 30
(mins) 47 87 36 65
Yield (%) 69 12 21 36
Table ST3: Yield of devices with MR ≥ 80%. The groups are listed based on their CFMS thickness, either 5 or 30. All were deposited at 1000 V.